Radiation Resistance of Teflon as a Filter Moderator Material
Journal of Nuclear Materials 304 (2002) 83–85
Letter to the Editors
Irradiation performance of polytetraﬂuoroethylene (Teﬂonâ )
in a mixed fast neutron and gamma radiation ﬁeld
Otto K. Harling *, Gordon E. Kohse, Kent J. Riley
MIT Nuclear Reactor Laboratory, 138 Albany Street, Cambridge, MA 02139, USA
Received 17 December 2001; accepted 1 April 2002
Samples of polytetraﬂuoroethylene have been irradiated with a mixed ﬁeld of fast neutrons and gamma rays using
the MIT Research Reactor. Dose levels from $0.3 to $50 Â 106 Gy for gamma and from $0.13 to 80 Â 104 Gy for fast
neutrons were used. Weight loss, ﬂuorine loss, and swelling were measured quantitatively. Subjective mechanical
property tests were also performed to assess embrittlement. Aside from high levels of embrittlement, no large changes,
J 1.5%, were observed in the properties which were assayed even at the highest doses. Ó 2002 Elsevier Science B.V. All
1. Introduction swelling or shrinkage appear to exist in the published
literature. Fluorine loss as a function of radiation dose
Our primary motivation for irradiation testing of has been reported by Ryan . In this paper we report
polytetraﬂuoroethylene (PTFE) (Teﬂonâ ) was related to post irradiation measurements of swelling, weight loss,
its applications in neutron ﬁlters used to produce high ﬂuorine loss and embrittlement for a range of doses
purity epithermal neutron beams, 1 eV K En K 10 keV, from $30 Â 106 to $5 Â 109 Rads. The lower range of
for neutron capture therapy applications [1–3]. The de- these doses overlaps the doses reached in previous
sirable neutronic properties for this application are pri- measurements and the higher range signiﬁcantly exceeds
marily related to the ﬂuorine content of the PTFE. High the doses used in Refs. [4–10]. Some of our results have
radiation doses from gamma rays and neutrons are ex- previously been published in a symposium proceeding,
pected in the ﬁlter application and it was desirable to which emphasized the neutronic performance of PTFE
demonstrate that the physical and chemical properties of for epithermal neutron beam production . The re-
the PTFE were suﬃciently stable for this application. In sults presented here also include substantially improved
particular, the swelling or shrinkage and the ﬂuorine loss fast neutron dosimetry.
should be limited to a few percent. Tensile properties are
not of great importance in this application as long as the
material does not crumble. 2. Irradiation and post-irradiation testing
Most previous irradiation performance studies of
PTFE have focussed on physical, electrical and me- A series of irradiations of PTFE samples were carried
chanical properties such as shear, tensile, elastic modu- out in the 5 MW, MIT Research Reactor. Samples were
lus, weight loss, gas evolution and electrical resistivity irradiated in mixed ﬁelds of fast neutrons and gamma
[4–9]. However, no results for irradiation-induced rays to several dose levels. Bars of virgin grade Teﬂonâ ,
about 0.6 cm square by 10 cm long were irradiated in a
pneumatic tube irradiation facility near the MITR’s core
Corresponding author. Tel.: +1-617 253 4201; fax: +1-617 tank. The gamma dose rate was approximately 3:3 Â 104
253 7300. Gy/min while the fast neutron ﬂux (E > 1 MeV) ranged
E-mail address: firstname.lastname@example.org (O.K. Harling). from 3:9 Â 1015 to 1:8 Â 1016 n/m2 s, corresponding to a
0022-3115/02/$ - see front matter Ó 2002 Elsevier Science B.V. All rights reserved.
PII: S 0 0 2 2 - 3 1 1 5 ( 0 2 ) 0 0 8 4 9 - 8
84 O.K. Harling et al. / Journal of Nuclear Materials 304 (2002) 83–85
dose rate range of approximately 1:2 Â 102 –5:4 Â 102 group were exposed to gamma doses of approximately
Gy/min. Sample temperature during irradiation was 1:6 Â 107 Gy and 1.2–5:5 Â 1020 n/m2 (5.9–27 Â 104 Gy)
determined to be in the range of 93–107 °C by using fast neutron dose. These samples were very brittle,
temperature indicating waxes . swelled 0–0.1% and had a ﬂuorine loss of <1.0%. Weight
Post-irradiation testing was performed to determine loss measurements for this dose group were inconclusive
the degree of swelling, weight changes, embrittlement due to the high probability of chipping the embrittled
and loss in ﬂuorine content. To assess swelling the sam- material during handling. At the fourth and highest dose
ple thickness was measured with a micrometer. Weight a sample was exposed to approximately 4:8 Â 107 Gy
changes were determined with a sensitive balance. Em- gamma and 1:6 Â 1021 n/m2 (79:5 Â 104 Gy) of fast neu-
brittlement was subjectively assessed by physical tests, tron dose. This sample was highly embrittled, exhibited
bending and cleaving. Assays of ﬂuorine content were swelling of $1% and ﬂuorine loss of K 1.5%. Weight
made by slow neutron activation analysis. Pre-irradia- loss measurements were inconclusive due to sample
tion and post-irradiation properties were assayed with chipping.
each type of test. The results of these irradiation tests of Teﬂonâ show
the embrittlement which has been observed by other
investigators. However, the current results also show
3. Results that only small levels of swelling, $1%, and K 1.5% of
ﬂuorine loss are experienced at gamma and fast neutron
The results of the irradiation tests are summarized in doses as high as 4:8 Â 107 Gy and 7:95 Â 105 Gy re-
Fig. 1 for four groups of samples which have been ex- spectively. The ﬂuorine loss is consistent with the results
posed to increasing levels of gamma and fast neutron reported in Ref.  and extends those results to 5Â
dose/ﬂuence. PTFE samples were, as expected, strongly higher dose. Although very severe embrittlement was
embrittled even at the lowest doses used in these tests, observed at the higher doses, the PTFE samples main-
approximately $3:4 Â 105 Gy gamma and 0.25–1:2 Â tained their shape, were self-supporting and did not
1019 n/m2 , (0.1–0:6 Â 104 Gy) fast neutrons. No dimen- degrade to a powder. Therefore, PTFE (Teﬂonâ ) ap-
sional changes, weight loss or ﬂuorine loss is observed pears to have adequate physical and chemical stability
for this group of samples. The intermediate dose group for use in neutron ﬁlter applications. The rectangle in
samples received approximately 3:7 Â 106 Gy gamma the middle left hand side of Fig. 1 shows the expected
and 0.28–1:2 Â 1020 n/m2 (1.4–6:1 Â 104 Gy) fast neu- lifetime radiation exposure for a high intensity epither-
trons. These sample were brittle, had weight loss of mal neutron beam currently in operation at the MIT
$0.1%, exhibited shrinkage in the 0–0.3% range and had Research Reactor. This shows that PTFE should per-
no measurable ﬂuorine loss. The samples in the third form satisfactorily in the neutron ﬁlter application
Fig. 1. Summary of the PTFE irradiation tests.
O.K. Harling et al. / Journal of Nuclear Materials 304 (2002) 83–85 85
provided of course that the accelerated tests reported  H. Kudoh, T. Sasuga, T. Seguchi, in: R.L. Clough, S.W.
here produce representative results for a PTFE appli- Shalaby (Eds.), Irradiation of Polymers: Fundamentals
cation where the dose rates are orders of magnitude and Technological Applications, American Chemical So-
lower than the dose rates used in the tests reported here. ciety, Washington, DC, 1996, p. 2.
 A. Chapiro, Radiation Chemistry of Polymeric Systems,
Funding for this project was provided by the US De-
John Wiley, New York, 1962, p. 527.
partment of Energy, Oﬃce of Science under contract  L.P. Yanova, A.B. Taulman, Deistvie Ionizirunyushchikh
numbers DE-FG02-97ER62489 for FCB construction Izluchenii na Neorganischeskie i Organicheskie Sistemy,
and DE-FG02-96ER62193 for facility design activities. Academy of Sciences of the USSR, Moscow, 1958, p. 314.
 V.S. Ivanov, Radiation Chemistry of Polymers, VSPBV,
The Netherlands, 1992, p. 177, 274.
References  M.H. Van de Voorde, C. Restat, Selection Guide to
Organic Materials for Nuclear Engineering, 49, CERN,
 W.S. Kiger III, S. Sakamoto, O.K. Harling, Nucl. Sci. Eng. Geneva, 1972, p. 72.
131 (1999) 1.  J.W. Ryan, Modern Plastics 31 (8) (1954) 148.
 S. Sakamoto, W.S. Kiger, O.K. Harling, Medical. Phys. 26  J.W. Ryan, Modern Plastics 31 (2) (1953) 152.
(9) (1999) 1979.  O.K. Harling, G. Kohse, K.J. Riley, S. Sakamoto, in: Haw-
 INEL BNCT Research Program Annual Report 1994, J.R. thorne et al. (Eds.), Frontiers in Neutron Capture Therapy,
Venhuizen, ed., Lockheed National Engineering Labora- Kluwer Academic/Plenum, New York, 2001, p. 363.
tory, Lockheed Idaho Technologies Company, Idaho  Tempil, Inc., Hamilton Blvd., S. Plainﬁeld, NJ 07080,
Falls, ID, November, 1995. USA.